Presentation on theme: "Chapter 9 – Solid Solutions and Phase Equilibrium"— Presentation transcript:
1 Chapter 9 – Solid Solutions and Phase Equilibrium The Science and Engineering of Materials, 4th ed Donald R. Askeland – Pradeep P. PhuléChapter 9 – Solid Solutions and Phase Equilibrium
2 Objectives of Chapter 9The goal of this chapter is to describe the underlying physical concepts related to the structure of matter.To examine the relationships between structure of atoms-bonds-properties of engineering materials.Learn about different levels of structure i.e. atomic structure, nanostructure, microstructure, and macrostructure.
3 Chapter Outline 9.1 Phases and the Phase Diagram 9.2 Solubility and Solid Solutions9.3 Conditions for Unlimited Solid Solubility9.4 Solid-Solution Strengthening9.5 Isomorphous Phase Diagrams9.6 Relationship Between Properties and the Phase Diagram9.7 Solidification of a Solid-Solution Alloy9.8 Nonequilibrium Solidification and Segregation
4 Section 9.1 Phases and the Phase Diagram Phase - Any portion including the whole of a system, which is physically homogeneous within it and bounded by a surface so that it is mechanically separable from any other portions.Gibbs phase rule - Describes the number of degrees of freedom, or the number of variables that must be fixed to specify the temperature and composition of a phase (2 + C = F + P, where pressure and temperature can change, 1 + C = F + P, where pressure or temperature is constant).P-T diagram - A diagram describing thermodynamic stability of phases under different temperature and pressure conditions (same as a unary phase diagram).
7 Design of an Aerospace Component Example 9.1Design of an Aerospace ComponentBecause magnesium (Mg) is a low-density material (ρMg = g/cm3), it has been suggested for use in an aerospace vehicle intended to enter the outer space environment. Is this a good design?Example 9.1 SOLUTION- In space the pressure is very low. Even at relatively low temperatures, solid magnesium can begin to change to a vapor, causing metal loss that could damage a space vehicle.- A low-density material with a higher boiling point (and, therefore, lower vapor pressure at any given temperature) might be a better choice.- Other factors to consider: In load-bearing applications, we should not only look for density but also for relative strength. Therefore, the ratio of Young’s modulus to density or yield strength to density could be a better parameter to compare different materials.
8 Example 9.2 Freeze Drying Synthesis of Ceramic Superconductors Many ceramic materials are made into powders using different oxides and carbonates (Chapter 14). This is because ceramics melt at too high a temperature and tend to exhibit brittle behavior. For example, the synthesis process for YBa2Cu3O7-x, a ceramic superconductor known as YBCO, involves mixing and reacting powders of yttrium oxide (Y2O3), copper oxide (CuO), and barium carbonate (BaCO3). The barium carbonate decomposes to BaO during the high temperature reactions and reacts with yttria and copper oxide to form different phases. Often, this process, known as the ‘‘oxide mix’’ technique, produces ceramic powders that are relatively coarse. Some other undesired phases may also form, and deleterious impurities (from processing or raw materials) may become incorporated in the product.
9 Example 9.2 (Continued)On the other hand, chemical techniques that make use of high-purity chemicals may offer a better product (most likely at a higher cost). One such chemical process, used in the food industry (e.g., coffee, spices, etc.) is freeze drying. For example, freeze-dried coffee is made by extracting coffee from beans and then evaporating the water from the coffee using freeze drying.An engineer decides to use water-based solutions to develop a freeze-drying synthesis of a YBCO superconductor. Using the unary phase diagram for water [Figure 9.3(a)], explain the different steps that could be followed to generate high-purity and chemically homogeneous powders of the YBCO superconductor.
11 Example 9.2 SOLUTION- Prepare a solution of nitrates of yttrium, copper, and barium in proper cation stoichiometry.- Remove the nitric acid (HNO3) and H2O without causing any melting by lowering the pressure to approximately 10-2 torr (point B).- Increase the temperature while maintaining the low pressure causing the ice and nitric acid to sublimate (solid vapor).- The mixed metal nitrate powder will then be heated carefully and the nitrates can be decomposed to form a ceramic powder.
12 Section 9.2 Solubility and Solid Solutions Solubility - The amount of one material that will completely dissolve in a second material without creating a second phase.Unlimited solubility - When the amount of one material that will dissolve in a second material without creating a second phase is unlimited.Limited solubility - When only a maximum amount of a solute material can be dissolved in a solvent material.Copolymer - A polymer that is formed by combining two or more different types of monomers usually with the idea of blending the properties affiliated with individual polymers, example DylarkTM a copolymer of maleic anhydride and styrene.
16 Section 9.3 Conditions for Unlimited Solid Solubility Hume-Rothery rules - The conditions that an alloy or ceramic system must meet if the system is to display unlimited solid solubility. Hume-Rothery’s rules are necessary but are not sufficient for materials to show unlimited solid solubility.Hume-Rothery rules:- Size factor- Crystal structure- Valence- Electronegativity
18 Example 9.3 Ceramic Solid Solutions of MgO NiO can be added to MgO to produce a solid solution. What other ceramic systems are likely to exhibit 100% solid solubility with MgO?Example 9.3 SOLUTIONFrom Appendix B, some other possibilities in which the cation has a valence of +2 include the following:
19 Example 9.3 SOLUTION (Continued) The percent difference in ionic radii and the crystal structures are also shown and suggest that the FeO-MgO system will probably display unlimited solid solubility. The CoO and ZnO systems also have appropriate radius ratios and crystal structures.
20 Section 9.4 Solid-Solution Strengthening Solid-solution strengthening - Increasing the strength of a metallic material via the formation of a solid solution.Dispersion strengthening - Strengthening, typically used in metallic materials, by the formation of ultra-fine dispersions of a second phase.
23 Example 9.4 SOLUTIONThe atomic radii and percent size difference are shown below:For atoms larger than copper—namely, zinc, aluminum, and tin— increasing the size difference increases the strengthening effect. Likewise for smaller atoms, increasing the size difference increases strengthening.
25 Section 9.5 Isomorphous Phase Diagrams Binary phase diagram - A phase diagram for a system with two components.Ternary phase diagram - A phase diagram for a system with three components.Isomorphous phase diagram - A phase diagram in which components display unlimited solid solubility.Liquidus temperature - The temperature at which the first solid begins to form during solidification.Solidus temperature - The temperature below which all liquid has completely solidified.
27 Example 9.5 NiO-MgO Isomorphous System From the phase diagram for the NiO-MgO binary system [Figure 9.10(b)], describe a composition that can melt at 2600oC but will not melt when placed into service at 2300oC.Figure 9.10 (b) The liquidus and solidus temperatures are shown for a Cu-40% Ni alloy.
28 Example 9.5 SOLUTIONTo identify a composition with a liquidus temperature below 2600oC, there must be less than 65 mol% MgO in the refractory. To identify a composition with solidus temperature above 2300oC, there must be at least 50 mol% MgO present.Consequently, we can use any composition between 50 mol% MgO and 65 mol% MgO.
29 Example 9.6 Design of a Composite Material One method to improve the fracture toughness of a ceramic material (Chapter 6) is to reinforce the ceramic matrix with ceramic fibers. A materials designer has suggested that Al2O3 could be reinforced with 25% Cr2O3 fibers, which would interfere with the propagation of any cracks in the alumina. The resulting composite is expected to operate under load at 2000oC for several months. Criticize the appropriateness of this design.
31 Example 9.6 SOLUTIONSince the composite will operate at high temperatures for a substantial period of time, the two phases—the Cr2O3 fibers and the Al2O3 matrix—must not react with one another. In addition, the composite must remain solid to at least 2000oC. The phase diagram in Figure 9.11 permits us to consider this choice for a composite.Pure Cr2O3, pure Al2O3, and Al2O3-25% Cr2O3 have solidus temperatures above 20000C; consequently, there is no danger of melting any of the constituents. However, Cr2O3 and Al2O3 display unlimited solid solubility. At the high service temperature, 2000oC, Al3+ ions will diffuse from the matrix into the fiber, replacing Cr3+ ions in the fibers. Simultaneously, Cr3+ ions will replace Al3+ ions in the matrix. Long before several months have elapsed, these diffusion processes cause the fibers to completely dissolve into the matrix. With no fibers remaining, the fracture toughness will again be poor.
32 Example 9.7 Gibbs Rule for Isomorphous Phase Diagram Determine the degrees of freedom in a Cu-40% Ni alloy at (a) 1300oC, (b) 1250oC, and (c) 1200oC.Example 9.7 SOLUTIONThis is a binary system (C = 2). Two components are Cu and Ni. We will assume constant pressure. Therefore, Equation 9-2 (1 + C = F + P) can be used as follows:(a) At 1300oC, P = 1, since only one phase (liquid) is present; C = 2, since both copper and nickel atoms are present. Thus:1 + C = F + P So, = F + 1 or F = 2
33 Example 9.7 SOLUTION (Continued) (b) At 1250oC, P = 2, since both liquid and solid are present; C = 2, since copper and nickel atoms are present. Now:1 + C = F + P So, = F + 2 or F = 1(c) At 1200oC, P = 1, since only one phase, solid, is present; C = 2, since both copper and nickel atoms are present. Again,1 + C = F + P So, = F + 1 or F = 2
36 Example 9.8 SOLUTIONThe vertical line at 40% Ni represents the overall composition of the alloy:- 1300oC: Only liquid is present. The liquid must contain 40% Ni, the overall composition of the alloy.- 1270oC: Two phases are present. The liquid contains 37% Ni and the solid contains 50% Ni.- 1250oC: Again two phases are present. The tie line drawn at this temperature shows that the liquid contains 32% Ni and the solid contains 45% Ni.- 1200oC: Only solid is present, so the solid must contain 40% Ni.
38 Example 9.9 SOLUTIONLet’s say that x = mass fraction of the alloy that is solid . Since we have only two phases, the balance of nickel must be in the liquid phase (L). Thus, the mass fraction of nickel in liquid will be 1 - x.Total mass of nickel in 100 grams of the alloy = mass of nickel in liquid + mass of nickel inSo, 100 (% Ni in alloy = [(100)(1 – x)](% Ni in L) + (100)[x](% Ni in )x = (40-32)/(45-32) = 8/13 = 0.62If we convert from mass fraction to mass percent, the alloy at 1250oC contains 62% a and 38% L. Note that the concentration of Ni in alpha phase (at 1250oC) is 45% and concentration of nickel in liquid phase (at 1250oC) is 32%.
44 Example 9.11 SOLUTIONFrom Figure 9.15, we determine the required composition of the alloy. To satisfy all of these conditions, we could use:Cu-90% Ni or Cu-33% to 60% NiWe prefer to select a low nickel content, since nickel is more expensive than copper. In addition, the lower nickel alloys have a lower liquidus, permitting castings to be made with less energy being expended. Therefore, a reasonable alloy might be Cu-35% Ni.
45 Example 9.11 SOLUTION (Continued) To produce this composition from the available melting stock, we must blend some of the pure nickel with the Cu-20% Ni ingot. Assume we wish to produce 10 kg of the alloy. Let x be the mass of Cu-20% Ni alloy we will need. The mass of pure Ni needed will be 10 - x.Since the final alloy consists of 35% Ni, the total mass of Ni needed will be:(10 Kg)( 35% Ni / 100%) = 3.5 Kg NiNow let’s write a mass balance for nickel. Nickel from the Cu-20% alloy + pure nickel added = total nickel in the 35% alloy being produced.0.2x x = 3.56.5 = 0.8xx = kg
46 Section 9.7 Solidification of a Solid-Solution Alloy Segregation - The presence of composition differences in a material, often caused by insufficient time for diffusion during solidification.
49 Section 9.8 Nonequilibrium Solidification and Segregation Coring - Chemical segregation in cast products, also known as microsegregation or interdendritic segregation.Homogenization heat treatment - The heat treatment used to reduce the microsegregation caused during nonequilibrium solidification.Macrosegregation - The presence of composition differences in a material over large distances caused by nonequilibrium solidification.Spray atomization - A process in which molten alloys or metals are sprayed using a ceramic nozzle.
51 Example 9.12 Nonequilibrium Solidification of Cu-Ni Alloys Calculate the composition and amount of each phase in a Cu-40% Ni alloy that is present under the nonequilibrium conditions shown in Figure 9.18 at 1300oC, 1280oC, 1260oC, 1240oC, 1200oC, and 1150oC. Compare with the equilibrium compositions and amounts of each phase.
53 Example 9.12 SOLUTIONWe use the tie line upto the equilibrium solidus temperature to calculate composition and percentages of phases as per the lever rule. Similarly, the nonequilibrium solidus temperature curve is used to calculate percentages and concentrations of different phases formed under nonequilibrium conditions.
55 Figure 9.19 (a) Microsegregation between dendrites can be reduced by a homogenization heat treatment. Counterdiffusion of nickel and copper atoms may eventually eliminate the composition gradients and produce a homogeneous composition. (b) Spray atomized powders of superalloys. (c) Progression of densification in low carbon Astroalloy sample processed using HIP. (Courtesy of J. Staite, Hann, B. and Rizzo, F., Crucible Compaction Metals.)